Two-Dimensional Dion-Jacobson Hybrid Lead Iodide Perovskites with Aromatic Diammonium Cations.
Li, Xiaotong; Ke, Weijun; Traoré, Boubacar; Guo, Peijun; Hadar, Ido; Kepenekian, Mikaël; Even, Jacky; Katan, Claudine; Stoumpos, Constantinos C.; Schaller, Richard D.; Kanatzidis, Mercouri G.; Journal of the American Chemical Society 141 (2019) 12880–12890; doi:10.1021/jacs.9b06398

data_4127723
_publ_section_title
;
 Two-Dimensional Dion-Jacobson Hybrid Lead Iodide Perovskites with
 Aromatic Diammonium Cations.
;
_journal_issue                   32
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              12880
_journal_page_last               12890
_journal_paper_doi               10.1021/jacs.9b06398
_journal_volume                  141
_journal_year                    2019
_chemical_formula_sum            'C8 H22 I10 N4 Pb3'
_chemical_formula_weight         2064.9
_space_group_IT_number           9
_space_group_name_Hall           'C -2yc'
_space_group_name_H-M_alt        'C 1 c 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      9
_symmetry_space_group_name_Hall  'C -2yc'
_symmetry_space_group_name_H-M   'C 1 c 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.920(9)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   45.091(5)
_cell_length_b                   9.0494(15)
_cell_length_c                   8.8654(10)
_cell_measurement_reflns_used    3598
_cell_measurement_temperature    293
_cell_measurement_theta_max      29.44
_cell_measurement_theta_min      2.22
_cell_volume                     3598.2(8)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_structure_refinement  JANA2006
_computing_structure_solution    JANA2006
_diffrn_ambient_temperature      293
_diffrn_detector                 'image plate (34 cm diameter)'
_diffrn_detector_area_resol_mean 6.67
_diffrn_measured_fraction_theta_full 0.99
_diffrn_measured_fraction_theta_max 0.99
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'IPDS Stoe'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1593
_diffrn_reflns_av_unetI/netI     0.0457
_diffrn_reflns_limit_h_max       61
_diffrn_reflns_limit_h_min       -61
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            16755
_diffrn_reflns_theta_full        29.2
_diffrn_reflns_theta_max         29.2
_diffrn_reflns_theta_min         1.82
_diffrn_source
'sealed X-ray tube, 12 x 0.4 mm long-fine focus'
_diffrn_source_current           40
_diffrn_source_power             2.00
_diffrn_source_voltage           50
_exptl_absorpt_coefficient_mu    22.587
_exptl_absorpt_correction_T_max  0.1181
_exptl_absorpt_correction_T_min  0.0190
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-SHAPE
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.8117
_exptl_crystal_description       'square plate'
_exptl_crystal_F_000             3496
_exptl_crystal_size_max          0.1396
_exptl_crystal_size_mid          0.1145
_exptl_crystal_size_min          0.0616
_refine_diff_density_max         8.45
_refine_diff_density_min         -6.03
_refine_ls_abs_structure_details
'  2964 of Friedel pairs used in the refinement'
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    7.96
_refine_ls_goodness_of_fit_ref   5.92
_refine_ls_hydrogen_treatment    constr
_refine_ls_number_constraints    99
_refine_ls_number_parameters     157
_refine_ls_number_reflns         6220
_refine_ls_number_restraints     26
_refine_ls_R_factor_all          0.1867
_refine_ls_R_factor_gt           0.1285
_refine_ls_shift/su_max          0.0448
_refine_ls_shift/su_mean         0.0036
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1663
_refine_ls_wR_factor_ref         0.1674
_reflns_number_gt                3470
_reflns_number_total             6220
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            ja9b06398_si_002.cif
_cod_data_source_block           3AMPYPb3I10
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/home/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_database_code               4127723